**warwick.ac.uk/lib-publications **

**Original citation: **

### Patrick, Christopher E., Kumar, Santosh, Balakrishnan, Geetha, Edwards, R. S. (Rachel Sian),

### Lees, Martin R., Mendive-Tapia, Eduardo, Petit , Leon and Staunton, Julie B.. (2017)

### Rare-earth/transition-metal magnetic interactions in pristine and (Ni,Fe)-doped YCo5 and GdCo5.

### Physical Review Materials, 1 (2). 024411.

**Permanent WRAP URL: **

### http://wrap.warwick.ac.uk/89994

**Copyright and reuse: **

### The Warwick Research Archive Portal (WRAP) makes this work by researchers of the

### University of Warwick available open access under the following conditions. Copyright ©

### and all moral rights to the version of the paper presented here belong to the individual

### author(s) and/or other copyright owners. To the extent reasonable and practicable the

### material made available in WRAP has been checked for eligibility before being made

### available.

### Copies of full items can be used for personal research or study, educational, or not-for-profit

### purposes without prior permission or charge. Provided that the authors, title and full

### bibliographic details are credited, a hyperlink and/or URL is given for the original metadata

### page and the content is not changed in any way.

**Publisher statement: **

### © 2017 American Physical Society

**A note on versions: **

### The version presented here may differ from the published version or, version of record, if

### you wish to cite this item you are advised to consult the publisher’s version. Please see the

### ‘permanent WRAP URL’ above for details on accessing the published version and note that

### access may require a subscription.

### and GdCo

5Christopher E. Patrick,1 _{Santosh Kumar,}1 _{Geetha Balakrishnan,}1 _{Rachel S. Edwards,}1

Martin R. Lees,1 _{Eduardo Mendive-Tapia,}1 _{Leon Petit,}2 _{and Julie B. Staunton}1,∗
1_{Department of Physics, University of Warwick, Coventry CV4 7AL, United Kingdom}

2

Daresbury Laboratory, Daresbury, Warrington WA4 4AD, United Kingdom

(Dated: July 10, 2017)

We present an investigation into the intrinsic magnetic properties of the compounds YCo5 and

GdCo5, members of the RETM5 class of permanent magnets (RE = rare earth, TM = transition

metal). Focusing on Y and Gd provides direct insight into both the TM magnetization and RE-TM interactions without the complication of strong crystal field effects. We synthesize single crystals of YCo5 and GdCo5 using the optical floating zone technique and measure the magnetization from

liquid helium temperatures up to 800 K. These measurements are interpreted through calculations based on a Green’s function formulation of density-functional theory, treating the thermal disorder of the local magnetic moments within the coherent potential approximation. The rise in magnetization with temperature of GdCo5is shown to arise from a faster disordering of the Gd magnetic moments

compared to the antiferromagnetically-aligned Co sublattice. We use the calculations to analyze the different Curie temperatures of the compounds and also compare the molecular (Weiss) fields at the RE site with previously-published neutron scattering experiments. To gain further insight into the RE-TM interaction we perform substitutional doping on the TM site, studying the compounds RECo4.5Ni0.5, RECo4Ni and RECo4.5Fe0.5. Both our calculations and experiments on powdered

samples find an increased/decreased magnetization with Fe/Ni-doping respectively. The calculations further reveal a pronounced dependence on the location of the dopant atoms of both the Curie temperatures and the Weiss field at the RE site.

I. INTRODUCTION

The discovery of the favorable magnetic properties of SmCo5 fifty years ago1 triggered a technological

revolu-tion based on rare-earth transirevolu-tion-metal (RE-TM) per-manent magnets.2In SmCo5, the strong magnetism of Co

combines with the large magnetocrystalline anisotropy
of localized Sm-4f electrons to form an excellent
perma-nent magnet. As well as having provided the blueprint
for the development of the now ubiquitous Nd-Fe-B
RE-TM magnet class,3 _{Sm-Co compounds still play an }

im-portant role in commercial applications due to their su-perior high-temperature performance.4 SmCo5 also

re-mains interesting from a fundamental viewpoint, since understanding precisely how the complicated interplay of localized and delocalized electrons affects the anisotropy and magnetization is a significant challenge for electronic structure theory.5

SmCo5 belongs to the RETM5 family of

perma-nent magnets which crystallize in the CaCu5 structure

(P6/mmm) whose unit cell is formed of alternating RETM2c/TM3g layers (Fig. 1).6 This relatively simple

crystal structure, paired with the diverse behavior ex-hibited by magnets with different RE,7make the RETM5

family an appealing playground for the investigation of RE-TM interactions. In particular, a hierarchy of com-plexity can be established beginning with RE = Y (i.e. a nonmagnetic RE with no 4f electrons), followed by RE = Gd (a half-filled 4f shell whose spherical symmetry re-moves a number of complications involving the spin-orbit interaction and crystal field [CF]), and finally a generic RE with a partly-filled 4f shell, like Sm. The different

FIG. 1. Ball-and-stick representation of the RETM5 crystal

structure, showing the RE site (purple) and two TM sublat-tices: TM2c (light gray, in plane with the RE) and TM3g (dark gray) where 2cand 3grefer to the Wyckoff positions.

energy scales involved in the interactions8_{allow this }

hier-archical approach to yield a quite general understanding of the TM-TM, RE-TM and RE-CF interactions respec-tively (the label “RE-CF” used in this sense denotes the interactions of the non-spherical 4f charge cloud with the crystal field). An early example of this approach is the empirical subtraction of the magnetization curve of YCo5 from other RECo5 compounds in order to observe

the RE magnetism.9

In order to lay the essential groundwork for the future study of compounds where RE-CF interactions are also important, here we concentrate on YCo5 and GdCo5.

par-ticular, by applying the disordered local moment (DLM)
picture10 _{we aim to understand the evolution of }

mag-netic properties with temperature, an aspect which is of obvious practical importance. To this end we have grown single crystals of YCo5and GdCo5using the

opti-cal floating zone technique (FZT) and measured the evo-lution of the magnetization up to 800 K. Our DFT-DLM calculations are able to explain both the contrasting tem-perature dependences of the two compounds and also the experimentally-observed higher Curie temperature of GdCo5. To further elucidate the RE-TM physics

under-lying these and other permanent magnets, we have also synthesized polycrystalline samples where Co was substi-tuted with Fe (Ni), which show an increase (decrease) in Curie temperature and magnetization. Our calculations reproduce this behavior, and further explore the depen-dence of these properties on the crystallographic site oc-cupied by the dopants. Indeed, the calculations find an unusual ferromagnetic RE-TM interaction between Gd and Fe when the atoms occupy nearest neighbor sites.

The rest of this manuscript is organized as follows. In section II we describe the experimental and compu-tational approach used in our study. In section III we report our findings, beginning with pristine YCo5 and

GdCo5 (section III A) and extending to the doped

sam-ples (section III G onwards). In section IV we summarize our results and present our conclusions.

II. EXPERIMENTAL AND THEORETICAL APPROACH

A. Experimental overview

Owing to its technological importance the RECo5

fam-ily has been the subject of extensive investigation for several decades, with experiments investigating the tem-perature dependence of magnetization and anisotropy of pristine RECo5 compounds.9,11–29 However, the growth

of single crystals remains challenging30,31and to the best of our knowledge our study represents the first successful attempt to grow single crystals of RECo5compounds

us-ing the optical FZT. Furthermore, while there are a num-ber of studies investigating specific cases of TM-doped RECo5 compounds,32–42 our study tackles both Ni and

Fe-doping on both YCo5 and GdCo5. By synthesizing

all compounds under the same experimental protocols, we can more rigorously compare trends measured across the series to our calculations.

B. Experimental approach

Polycrystalline samples of RECo5−xNix(RE = Y, Gd,

x = 0, 0.5, 1.0) and YCo4.5Fe0.5 were synthesized by

arc melting the constituent elements in the appropriate proportions on a water-cooled copper crucible in an ar-gon atmosphere. The ingots were melted, flipped and

remelted to ensure homogeneity. No significant changes in weight were observed after melting. Structural char-acterization was performed by recording powder x-ray diffraction (XRD) patterns of the as-cast samples using a Panalytical Empyrean x-ray diffractometer with a Co target. Single crystals of YCo5 and GdCo5 were grown

using a four-mirror Xenon arc lamp optical image fur-nace (CSI FZ-T-12000-X VI-VP, Crystal Systems Inc., Japan) using the floating zone technique. The polycrys-talline rods for the crystal growth were synthesized by arc melting. The single crystals obtained were aligned us-ing a backscattered X-ray Laue system (Photonic-Science Laue camera). Platelet-shaped crystal samples with the crystallographicc axis normal to the plane of the plates were obtained from the as-grown crystal boules. The measured lattice constants are reported in Appendix A. Magnetization measurements were carried out using a Quantum Design Magnetic Property Measurement Sys-tem (MPMS) superconducting quantum interference de-vice (SQUID) magnetometer. An oven option was used for measurements between 400 and 800 K. Magnetiza-tion measurements on the single crystals were performed with the applied magnetic field along the easy axis of magnetization so as to obtain the saturated moment val-ues. Below 400 K the data were collected at intervals of 10 K, while above 400 K the data were recorded while warming at 10 K/minute. In the case of the doped poly-crystalline samples, the magnetization versus field curves were recorded using powder samples, with the grains free to rotate under the influence of the magnetic field, so as obtain a best estimate of the saturated magnetic mo-ments.

C. Theoretical overview

Following on from theoretical studies of RECo5

compounds based on experimentally-parameterized
CF-models,9,14,18–22,25,27,36,42–45 first-principles
investiga-tions became possible thanks to developments in
density-functional theory.5,46,47 _{A greater number of }

first-principles studies of YCo548–63 can be found compared

to GdCo5,5,23,64,65 presumably due to the difficulty of

finding an approximate exchange-correlation functional capable of describing the localized Gd-4f electrons in DFT. However, most of these studies were performed in a conventional wavefunction-based framework, which is best suited to describing pristine systems at zero tem-perature. Although dopants can be modeled within this framework via calculations on supercells51,52,55,56,60 or by using virtual atoms,50,54the former approach quickly becomes costly in terms of size convergence while the latter cannot capture the full chemistry of the problem. Meanwhile the calculation of finite-temperature proper-ties in a wavefunction-based framework is generally lim-ited to obtaining critical temperatures based on an as-sumed Heisenberg model and pairwise interactions.53,60

Korringa-Kohn-Rostocker multiple-scattering formulation of
DFT66 _{combined with the coherent potential }

ap-proximation (KKR-CPA)67 _{and the disordered local}

moment picture,10 _{which reformulates the problem of}

compositional and thermal magnetic disorder in terms of impurity scattering. Ref. 59 used this approach to study the zero-temperature properties of (Al,Si)-doped YCo5, while Ref. 61 investigated the finite temperature

properties of pristine YCo5. The current study combines

the computational machinery of the KKR-CPA, the DLM picture, and the local self-interaction correction developed in Ref. 68 to tackle the full problem of the temperature-dependent magnetic properties of pristine and transition-metal-doped YCo5and GdCo5.

D. Theoretical approach

We follow closely the computational approach de-scribed in Ref. 61 and refer the reader to that and other works10,69–71for a detailed presentation of the underlying theory. Here we define and describe the key quantities used in our analysis. The technical details of our calcu-lation are reported in Appendix B.

The key concept in the DLM picture is the assignment
of a local magnetic moment µi to each magnetic ion,
which we label by the subscript i. This local moment
undergoes fluctuations on the timescale associated with
spin-wave excitations, but is stable over the much shorter
timescale associated with electron motion.10 _{Introducing}

the unit vectors eˆi = µi/µi to denote the orientations

of the local moments, a “good” local moment system is one where the magnitudes {µi} do not depend strongly on the orientations {ˆei}.70 The statistical mechanics of such a system is determined by the thermodynamic po-tential Ω({eˆi}) which in principle could be obtained from finite-temperature constrained DFT on a large supercell containing many local moments.10However, the number of such calculations required to adequately sample the large configurational space spanned by all of the possi-ble orientations {ˆei} makes such a direct approach in-tractable.

To proceed, we instead approximate the statistical me-chanics of the local moments with that of an auxiliary system, defined in terms of a model potential

Ω0({eˆi}) =−

X

i

hi·eˆi. (1)

The vectors{hi}are parameters of the model with units of energy; they play the role of molecular fields expe-rienced by the local moments, and we refer to them as “Weiss fields”. Although not written explicitly, the Weiss fields depend on temperature. The number of dis-tinct Weiss fields can be chosen to equal the number of crystallographically-distinct sites in the unit cell; how-ever, we emphasize that the sum in equation 1 is over all of the local moments, distributed over the entire crystal.

The potential of equation 1 yields a probability distri-bution for observing a set of local moment orientations

{eˆi}as

P0({eˆi}) =

Y

i

1 Z0i

exp[λi·eˆi] (2)

withZ0i = (4π/λi) sinh(λi), and we have introduced the

dimensionless quantitiesλi =βhi (where 1/β =kBT).

The thermal averages of certain quantities with respect to the model probability distributionP0 can be performed

analytically, e.g. the thermally-averaged orientation of a local momentmi(T) =heˆii0,T:

mi(T) =

Z

deˆieˆi

exp[λi·eˆi] Z0i

Y

j6=i Z

deˆj

exp[λj ·eˆj] Z0j

=λˆiL(λi) (3)

withL(λi) = coth(λi)−1/λi. mi(T) serve as local order parameters which vanish above the Curie temperature. The integrations are over the angular variables (θi, φi)

whereeˆi= (sinθicosφi,sinθisinφi,cosθi).

The link between the model parameters{hi} and the exact potential Ω({eˆi}) is established through use of the thermodynamic inequality10

F(T)≤F0(T)− hΩ0i0,T+hΩi0,T. (4)

Here F is the exact, unknown free energy. while F0 is

the free energy calculated with the model potential (an analytical function of the Weiss fields). The thermal av-erageshi0,T of the exact and model potentials are

calcu-lated with respect to the model probability distribution, emphasized by the 0 subscript. We define the optimal Weiss fields to be those which minimize the right hand side of equation 4. Performing the minimization yields

hi=−∇mihΩi0,T (5)

which can be equivalently written as an integral expression,10

hi=− 3 4π

Z

deˆihΩie0ˆ,Ti eˆi (6)

where hieˆi

0,T denotes a partial thermal average, i.e. the

appropriately-weighted integration over all local moment orientations excepteˆi.

Equation 6 is the expression used to evaluate the Weiss fields within the KKR-CPA formalism. One can draw the analogy with the simulation of alloys, where the local mo-ment disorder determined by the probability exp[λj·eˆj] is replaced with compositional disorder determined by a probability (concentration)cX. The CPA was originally

developed with the alloy problem in mind,66 _{and its }

coherent potential approximations. More details on the scattering theory underlying the evaluation of equation 6 are given e.g. in Ref. 61.

Since the Weiss fields themselves determine the prob-ability distribution used in the partial thermal average, equation 6 must be solved self-consistently. Indeed the critical (Curie) temperature TC for the onset of

mag-netic order is the highest temperature at which such self-consistent solutions can be found. Once the Weiss fields have been determined at a particular temperature, the model probability distribution P0 can be fed into

addi-tional KKR-CPA calculations to calculate thermal aver-ages of spin and orbital moments (and in principle other quantities such as the torque)69ashAi0,T, whereAis the

appropriate quantum mechanical operator.

III. RESULTS AND DISCUSSION

A. Magnetization vs. temperature of pristine YCo5

and GdCo5

We begin our study with pristine YCo5 and GdCo5.

The experimentally-determined magnetization vs. tem-perature (MvT) curves are shown in Fig. 2(a). These data were measured for our single crystals in an applied field of 1 or 2 T directed along the easy c-axis for tem-peratures below and above 400 K, respectively. As we discuss in Sec. III H, this field is sufficient to saturate the magnetization. We see from Fig. 2(a) that YCo5behaves

like an ordinary ferromagnet, with a monotonic decrease in magnetization per formula unit from 8.41µB at 4 K

to 6.38µB at 700 K. The magnetization of GdCo5

mean-while increases, from 1.74µB at 4 K to 3.21µB at 700 K.

For the behavior of the magnetization at higher
temperatures we refer to previously-reported
measurements,9,12,15 _{which show the magnetization}

of GdCo5 to start decreasing at temperatures in the

region of 700–800 K (a lower value of 600 K was found in Ref. 14). The reported Curie temperatures9,11,12,14,15 for GdCo5 fall in the range 1000–1030 K compared to

the lower range of 980–1000 K9,25,26_{reported for YCo}

5.

The review article of Ref. 72 gives values of 1014 K and 987 K for theTC of GdCo5 and YCo5 respectively.

Our calculatedMvT curves for YCo5 and GdCo5 are

shown in Fig. 2(b). Pleasingly, we see the same contrast-ing behavior between the compounds as observed experi-mentally. Our calculatedTCvalues are 885 and 940 K for

YCo5 and GdCo5respectively, while the 0 K

magnetiza-tions are calculated to be 8.64µB and 1.29µB. Table I

gives the decomposition of the magnetization into local spin and orbital moment contributions. As shown in Ta-ble I and as realized from early experiments,13 the RE and TM sublattices align antiferromagnetically, account-ing for the∼7µB difference between YCo5 and GdCo5.

YCo5 GdCo5

µRE — -7.32/-0.01

µCo2c 1.62/0.15 1.57/0.15

µCo3g 1.64/0.06 1.67/0.05

µCo_{3}_{g}0 1.63/0.08 1.65/0.07

µTot,calc 8.64 1.29 µTot,exp 8.41a 1.74a

µTot,exp 8.3b8.3c8.13d7.9e 1.55c1.72f 1.68g 1.42h

a_{Current work, 4 K, optical FZT}

b_{Ref. 25, 0 K, r.f. melting + heat treatment + grinding}
c_{Ref. 9, 4 K, r.f. melting + heat treatment + grinding}
d_{Ref. 24, 0 K, induction zone melting + grinding}

e_{Ref. 26, 0 K, plasma jet melting + heat treatment + grinding}
f_{Ref. 23, 5 K, r.f. melting + heat treatment + grinding}
g_{Ref. 17, 12 K, arc melting + grinding}

h_{Ref. 15, 0 K, plasma jet melting + heat treatment + grinding}

TABLE I. Magnetic moments in µB (per atom or formula unit) for pristine YCo5 and GdCo5. The calculations were

performed at 0 K for magnetization along the [101] direction. The experimental values have been measured by us or re-ported previously in the literature; note the 0 K values were obtained by extrapolation. The calculations have been re-solved into spin/orbital contributions with the Co atoms la-beled as in Fig. 1; note that the magnetization breaks the symmetry of the 3gsublattice, giving rise to a distinct con-tribution (3g0) from the Co atom at the 01

2 1

2 position.

B. Comparison of calculations and experiment

Table I also lists magnetizations measured by us and reported in previous literature on single crystals. It is apparent that the calculations find a larger magnetiza-tion for YCo5 and smaller one for GdCo5 than

mea-sured experimentally. However, the size of the discrep-ancy (0.4µB) is of the same magnitude as the change

in magnetization on applying an empirical orbital po-larization correction (0.5–0.8µB/f.u.48,49,51), the size of

the induced moment on Y (∼0.3µB,49,51 which we

disre-gard) and the variation of the magnetization depending on the choice of spherical approximation for the poten-tial (∼0.2 µB).49 Therefore we find the current level of

agreement between calculated and experimental magne-tizations to be acceptable. Comparing our experimental magnetizations to previously-reported values we find our values to lie in at the higher end of the range. However, as emphasized by Table I our study is unique using the optical FZT to synthesize the samples.

Regarding TC, the calculations reproduce the

experi-mental ordering of YCo5 and GdCo5 but the calculated

values are smaller than the experimentally-reported ones by approximately 100 K. Usually one would expect an overestimate ofTC in a mean-field approach. A possible

0 200 400 600 800 1000 0.0

2.0 4.0 6.0 8.0 1

T(K)

M

(

/f.u.)

µB

0 200 400 600 800 1000

0.0 2.0 4.0 6.0 8.0

T(K)

M

(

/f.u.)

µB

FIG. 2. Magnetization vs temperature (a) measured on single-crystal samples and (b) calculated in the DLM picture, for YCo5

(green) and GdCo5 (blue). The straight lines connecting points in (b) are guides to the eye.

600 700 800 900 1000

0.0 1.0 2.0 3.0

T(K)

M

(

/f.u.)

µB

FIG. 3. Magnetization calculated for GdCo5 using the

300 K lattice parameters (solid line, larger circles; cf. Fig. 2) or using the temperatudependent lattice parameters re-ported in Ref. 73 (dotted line, smaller circles). Note that the temperature-dependent lattice data points>950 K were all calculated using the same lattice parameters, measured at 1000 K in Ref. 73.

so conversely a calculation using a more accurate poten-tial might be expected to yield increased values of TC.

Unfortunately such full-potential calculations are not yet feasible within our computational framework.

An interesting additional consideration is the role of magnetostructural interactions. The data in Fig. 2(b) were calculated using the lattice constants measured at 300 K as reported in Refs. 73 and 74, namely a, c = 4.979, 3.972 ˚A for GdCo5 anda, c = 4.950, 3.986 ˚A for

YCo5. For GdCo5 we have investigated the effect of

lat-tice thermal expansion, by recalculating the magnetiza-tion at temperatures>600 K using the lattice parameter data given in Ref. 73. The comparison of magnetizations obtained for the fixed or expanding lattices are shown in Fig. 3. When lattice expansion is taken into account, the calculatedTCincreases by 42 K to 982 K. The sensitivity

of magnetic coupling to the lattice parameters is explored further in Sec. III D.

As a general note, we see that in the T → 0 limit, the gradients of the experimentalMvT curves go to zero

0 200 400 600 800 1000

0.0 2.0 4.0 6.0 8.0

T(K)

M

(

/f.u.)

µB

|M |Gd MCo

FIG. 4. Decomposition of the magnetization of GdCo5(faint

solid blue line) into contributions from the Gd and Co sublat-ticesMGdandMCo(dotted lines, small circles). Note that the sublattice magnetizations point antiparallel, so the resultant magnetization isMCo− |MGd|. The calculated magnetization of YCo5(green solid line) is also shown for comparison.

whilst those of the calculated curves do not. This behav-ior is a simple consequence of us using a classical rather than quantized expression to describe the statistical me-chanics of the local moments (equation 1).

C. The disordering of Gd in GdCo5

In order to better understand the temperature evolu-tion of the magnetism in GdCo5 it is instructive to

de-compose the total magnetization into contributions from the antialigned Gd and Co sublattices, as shown in Fig. 4. First we note that below 400 K, the Co contributionMCo

is indistinguishable from theMvT curve of YCo5,

show-ing that replacshow-ing Y with Gd (i.e. movshow-ing from a non-magnetic to non-magnetic RE) has a negligible effect on the TM ordering. This observation is in agreement with the established hierarchy of interaction strengths in RE-TM magnets11 and justifies the practice of subtracting the YCo5 curve from RECo5 measurements to observe the

-10 0 10 20 30

J(

m

R

y)

2c-2c

2c-3g

3g-3g

Co-Co Gd-Co2c

Gd-Co3g Gd-Gd

FIG. 5. Calculated values of Jij in the high-temperature expansion of equation 7 for GdCo5 (blue) and YCo5 (green).

The empty bars are the values ofJijcomputed for YCo5using

the lattice parameters of GdCo5 (see text).

discussed in Sec. III D the RE does have a noticeable effect on the TM sublattice at higher temperatures.

Now considering the Gd contribution, we see the magnitude of the magnetization |MGd| decreases more

quickly with temperature than MCo. As a result the

total magnetizationMCo− |MGd|increases with

temper-ature. As shown in Fig. 4 the decrease in |MGd| is

ef-fectively linear up to temperatures of 800 K, whileMCo

displays Brillouin function behavior. Consequently there is a temperature (∼600 K) where the gradients of MCo

and|MGd|are equal, corresponding to a peak in the total

magnetization, before MCo undergoes a faster decrease

close toTC. In Sec. III F we reexamine this behavior in

terms of the Weiss field at the RE site and compare to low-temperature experimental data.

D. Order parameter expansion of Ω0

The relative strengths of the TM-TM, TM and RE-RE interactions can be quantified by expanding the cal-culated potential energyhΩi0,T in terms of order

param-eters describing the thermally-averaged local moment at the different sublattices (mi; equation 3). Close to TC

(mi →0) the expansion can be truncated at second

or-der, i.e.:

hΩi0,T ≈

−1

2J2c−2cm

2

Co2c−J2c−3gmCo2cmCo3g

−1

2J3g−3gm

2

Co3g

−1

2JGd−Gdm

2 Gd

−JGd−Co_{2}_{c}mGdmCo2c−JGd−Co3gmGdmCo3g
(7)

where we have decomposed the Co contribution into the two inequivalent 2c and 3g sublattices (Fig. 1), and as-sumed collinear magnetization of the sublattices. Only

the terms in parentheses are required for YCo5.

Differen-tiation of equation 7 with respect tomiyields expressions

for the Weiss fields through equation 5, conveniently ex-pressed in matrix form:

hCo2c hCo3g hGd

=

J2c−2c

2

J2c−3g

2

JGd−_{Co2}_{c}
2
J2c−3g

3

J3g−3g

3

JGd−_{Co3}_{g}
3

JGd−Co2c JGd−Co3g JGd−Gd

mCo2c mCo3g mGd

.

(8) The denominators of 2 and 3 account for the multiplic-ities of the 2c and 3g positions. We then obtain theJij

coefficients from a least-squares fit of the calculated{hi}

values from a training set of {mi} (equivalently, {λi}), and plot them in Fig. 5. It is essential to stress that the Jij values are not simply describing pairwise

inter-actions, but rather should be thought of as coefficients in the rather general expansion ofhΩi0,T in equation 7.

This point is discussed further in Ref. 75.

Initially focusing on GdCo5 (blue bars in Fig. 5), we

first note the negative values ofJGd−Co2c andJGd−Co3g, as expected for antiferromagnetic alignment. The RE-RE interaction quantified byJGd−Gdis ferromagnetic but

negligibly small, i.e. the RE ordering is driven by RE-TM interactions. Interestingly, JGd−Co3g is 4.5 times larger than JGd−Co2c, showing that the dominant RE-TM in-teraction is not between in-plane nearest neighbors, but rather between the RE and the adjacent pure Co planes. It follows that substituting Co at the 3gpositions should have a greater effect on the RE than at the 2cpositions, a hypothesis that we test in Sec. III J.

Turning to the TM-TM interaction in GdCo5, again

we find the largestJij to correspond to interplanar

in-teractions, i.e.J2c−3g. The in-plane interactionsJ2c−2c,

J3g−3g are also ferromagnetic but smaller by J2c−3g by

factors of 5 and 2, respectively. Comparing theseJij

val-ues with those found for YCo5(green filled bars in Fig. 5)

we find the same ordering of values and similar magni-tudes, but the dominant J2c−3g coefficient of GdCo5 is

larger by 2.4%.

Given that the values of Jij determineTC (discussed

in the following section), we investigated the origin of the difference inJ2c−3g by performing a calculation on YCo5

using the lattice parameters of GdCo5. This procedure

amounts to increasing theaparameter by 0.5% and
re-ducing the c parameter by 0.4%.73,74 _{The resulting} _{J}

ij

values are shown as the empty green bars in Fig. 5. We see that the respective increase and decrease in a and c coincide with weakened in-plane interactions (J2c−2c,

J3g−3g). However, the interplanar interaction is

strength-ened by 2.9%, leading us to attribute the difference in J2c−3g between GdCo5and YCo5 to be structural in

0.0 0.5 1.0 0

100 200 300

mCo

0 200 400 600 800 1000

0 100 200 300

Temperature(K)

h

/

(T

)

### µ

GdG

d

FIG. 6. The molecular field on Gd in GdCo5. The open

circles show the calculated Weiss fields divided by the local moment magnitudes as a function of temperature. The in-set contains the same data as a function of the average Co order parameter. The dashed line shows the expected Weiss field based on theJexpansion of equation 7 and parameters shown in Fig. 5. The open square with error bars in the main panel denotes the molecular field measured by inelastic neu-tron scattering experiments at 20 K as reported in Ref. 76.

E. Calculation of TC fromJij

Equation 8 can be used to calculate TC by replacing

mi = L(λi) = L(βhi) and using the mi → 0 limit,

L(x) → x

3. Equation 8 then reduces to an eigenvalue

problem, with the smallestβ corresponding toTC. This

approach allows the analysis of the difference in TC

be-tween GdCo5 and YCo5. For instance, taking the Jij

values obtained for YCo5and then replacingJ2c−3g with

the larger value obtained for GdCo5 increases the

calcu-lated TC from 885 K to 900 K. Further replacingJ2c−2c

andJ3g−3g gives a further increase inTCto 906 K.

It follows that the remaining 60% of the increase inTC

observed for GdCo5(34 K, to 940 K) must be attributed

to the RE-TM and/or RE-RE interaction. We find that the small value ofJGd−Gd means that the RE-RE

inter-action accounts for less than 1 K of the difference, so it is the RE-TM interaction, especially the interplanar interaction characterized by JGd−Co3g, which is respon-sible. Therefore according to the calculations, although the RE-TM interaction does not affect the Co sublattice magnetization below 400 K (Fig. 4), the interaction is essential to understanding the higherTCof GdCo5.

F. Weiss field on Gd

In Fig. 6 we plot the temperature evolution of hGd,

the calculated Weiss field on Gd in GdCo5. Sincehi has

units of energy (equation 1) we convert to a field in tesla by dividing by the calculated local moment magnitude µGd, which varies from 7.30 to 7.05µB from T = 0 K to

TC. The inset plots the same data against the averaged

Co order parameter,mCo= (2mCo2c+ 3mCo3c)/5. The dashed line in Fig. 6 shows the expected behavior ofhGd according to equation 8. By construction this fit

is accurate close toTC, but at temperatures below 600 K

deviations are observed, such thathGdis no longer linear

in mCo (inset). To accurately reproduce the calculated

Weiss field at the RE site at these temperatures it is
nec-essary to include higher-order terms75 _{in the expansion}

of equation 7, preventing a straightforward mapping to a Heisenberg-like Hamiltonian.

Although the Weiss fields were introduced as
parame-ters as a means of modeling the local moment statistics,
it is reasonable to ask how they compare to the exchange
field at the RE site which can be measured via inelastic
neutron scattering (INS).76 _{Therefore in Fig. 6 we also}

plot the value of 236±8 T at 20 K which was measured in the INS experiments of Ref. 76. The excellent agree-ment with the calculated values of hGd/µGd is perhaps

fortuitous and certainly sensitive to the spherical
approx-imation to the potential,23 _{but nonetheless gives us }

con-fidence in the validity of the local moment description of the RE magnetism.

G. Substitutional doping of transition metals I: TM sites

We now go beyond the pristine RECo5 compounds

and consider substitutional doping of the transition met-als. We have investigated both experimentally and com-putationally the replacement of Co with its neighbor-ing elements Fe and Ni, considerneighbor-ing the compounds RECo4.5Ni0.5, RECo4Ni and RECo4.5Fe0.5. These low

dopant concentrations were chosen to avoid
compli-cations arising from structural modification through
doping74_{and the low solubility of Fe.}35,39_{Even so, due to}

this low solubility we were unable to synthesize a single-phase sample of GdCo4.5Fe0.5.

Previous experimental studies34,37,38attempted to de-termine whether the dopants preferentially occupy 2c or 3g sites (Fig. 1) or are distributed equally among the TM sublattices. The neutron diffraction experiments of Ref. 34 on Ni-doped YCo5found a preference for Ni

sub-stitution at 2csites (with 2c/3goccupancies of 0.16/0.06 for YCo4.5Ni0.5 and 0.29/0.14 YCo4Ni). For Fe-doped

YCo5 we are unaware of similar neutron measurements,

but the study of the related compound ThCo5in Ref. 37

found a preference for Fe-substitution at 3g sites (2c/3g occupancies of 0.2/0.5 for YCo3Fe2). On the other hand

Ref. 38 argued that the evolution of lattice parameters of YCo5 as a function of Fe-doping was consistent with

preferential substitution at 2c sites.

We have calculated the ground-state (zero tempera-ture) energies of RECo4.5T0.5, T = Ni or Fe, where the

0

-1

-2

-3

-4

E

ne

rg

y (

m

R

y/

f.u

.) RCo Ni4.5 0.5 RCo Fe4.5 0.5

FIG. 7. Calculated energetics of doping of GdCo5 (blue) or

YCo5 (green) by substituting at a Co2csite. They-axis zero corresponds to the energy per formula unit when the dopant is substituted at a Co3gsite, i.e. negative bars imply the dopant is more stable sitting at a Co2c site.

-1.0 0.0 1.0

0.0 2.0 4.0 6.0 8.0 10.0

Change in electron count w.r.t. RCo_{5}

M

(

/f.u.)

µB

RCo4.5Fe0.5 RCo5 RCo4.5Ni0.5 RCo4Ni

FIG. 8. Low temperature magnetizations of doped RECo5

compounds. The crosses show the magnetization of powdered samples in a field of 7 T at 5 K for Fe or Ni-doped YCo5

(green) and GdCo5 (blue). The circles and squares are the

magnetizations calculated where the dopants have been sub-stituted either at Co2cor Co3g sites respectively.

CPA calculations, 2c-substitution is more stable for both Ni and Fe-doping of both GdCo5 and YCo5 (blue and

green bars) Interestingly, there is a notable difference in the energetics of Fe-doping between GdCo5 and YCo5.

As discussed in Sec. III J this difference is due to a mag-netic energy penalty in placing Fe at 2csites when Gd is present.

Although the CPA calculations support 2c-ordering, the different conclusions drawn based on experiments37,38 may indicate a dependence on sample preparation routes. Therefore in order to keep our study general, in the fol-lowing we present calculations for both 2c and 3g pref-erential doping. We view these calculations as limiting cases, with the experimentally-realized situation lying somewhere in between.

H. Substitutional doping of transition metals II: Magnetizations

In Fig. 8 we present the saturation magnetizations measured and calculated for the doped RECo5

com-pounds. As we might expect, the behavior with doping

0.0 1.0 2.0 3.0 4.0 5.0 6.0 7.0

6.0 6.5 7.0 7.5 8.0 8.5

H(T)

µ0

M(

/f.u.)

µB

FIG. 9. Magnetization vs. applied field measured at 5 K for single crystal YCo5 (green line, filled circles), polycrystalline

(powdered) YCo5(green line, crosses), YCo4.5Ni0.5(gray line,

squares) and YCo4.5Fe0.5 (brown line, empty circles).

of GdCo5 and YCo5 is very similar. The general trend

is of an increase in magnetization with Fe-doping and a decrease with Ni-doping. This behavior is consistent with a rigid-band picture, noting that in YCo5 the

d-band is essentially full in the majority-spin channel and partially occupied in the minority channel;58 therefore increasing the electron count (through Ni-doping) fur-ther populates the minority-spin channel and decreases the overall moment, and vice versa for Fe-doping. The calculated magnetizations for the dopants occupying 2c or 3g sites (circles and squares in Fig. 8) are very simi-lar. The supercell calculations of Ref. 56 found the same behavior, again consistent with the rigid band model.

We now compare the magnetic moments for the poly-crystalline (powdered) samples of the pristine compounds (YCo5 and GdCo5) presented in Fig. 8 with the values

obtained for the magnetic moments of the single crystals given in Table I. For example, we note that the moment value for the polycrystalline YCo5 is 0.23µB/f.u. lower

than the value obtained for the YCo5 single crystal. In

order to explain this small difference, we focus our at-tention on the isothermal magnetization plots shown in Fig. 9 obtained at T = 5 K for all the polycrystalline (Fe, Ni)-doped YCo5 samples, where for comparison we

also plot the magnetization of the YCo5 single crystal

(green line). During the measurement process, the mag-netic field was reduced from 7 to 0 T and the magne-tization data were recorded at several field values. It is apparent that none of theMvH curves for the poly-crystalline materials saturate, even at a field of 7 T. In contrast, theMvH curve for the single crystal saturates aboveµ0H = 1 T. This demonstrates that it is easier to

saturate the magnetization of a single crystal (when H is applied along the easy axis of magnetization). For a polycrystalline sample of doped or pure YCo5 made up

-1.0 0.0 1.0 700

800 900 1000 1100

Change in electron count w.r.t. RCo_{5}

T (K)C

RCo4.5Fe0.5 RCo5 RCo4.5Ni0.5 RCo4Ni

FIG. 10. Curie temperatures calculated for YCo5 (green)

and GdCo5 (blue) for different doping concentrations, where

the dopants have been substituted either at Co2c (circles, dashed lines) or Co3g (squares, solid lines) sites.

situation is even more complex due to its ferrimagnetic ordering, which can lead to non-collinear Gd and Co spins when the applied field is not parallel to the easy axis.19 We have also observed that using solid rather than pow-der polycrystalline samples of YCo5 leads to even lower

values for the magnetic moment at the same H and T

(data not shown here). Nevertheless, using powder sam-ples one can obtain data that can be used to identify trends, e.g. the variation in the saturation magnetization with doping within a sample series, and the saturation moments obtained lie within a few percent of the single crystal values.

I. Substitutional doping of transition metals III: TC

In Fig. 10 we present the calculated Curie tempera-tures for the doped compounds. The variations in TC

with doping are found to be very similar for RE=Gd and Y, displaying the same∼60 K offset as observed for the pristine case and discussed in Sec. III E. However, unlike the magnetization plotted in Fig. 8, theTCvalues show

a pronounced dependence on whether the dopants are substituted at the 2c or 3g sites. The largest variations in TC occur when the dopants occupy the 2c sites, e.g.

increasing by 124 K for YCo4.5Fe0.5 and decreasing by

95 K for YCo4.5Ni0.5. However, doping with Fe on the

3g sites only raisesTC by 5 K for YCo4.5Fe0.5.

Further insight into the behavior ofTCcan be obtained

by extending the analysis of Sec. III D. The appropriate modification of equation 8 is

hCo2c hCo3g hT

hGd

=

c2cJ2c−2c

2

c3gJ2c−3g

2

cTJ2c−T

2

JGd−Co2c

2 c2cJ2c−3g

3

c3gJ3g−3g

3

cTJ3g−T

3

JGd−Co3g

3 c2cJ2c−T

n

c3gJ3g−T

n

cTJT−T

n

JGd−T

n

c2cJGd−Co2c c3gJGd−Co3g cTJGd−T JGd−Gd

mCo2c mCo3g mT

mGd

(9)

where n is the multiplicity of the dopant sites (2 or 3 for 2c or 3g doping, respectively). Removing all terms involving Gd gives the expression for YCo5. For the

compound RECo5−xTx, the dopant concentration cT is

given byx/n, while the Co concentrations (c2c, c3g) equal

(1−cT,1) for 2c-doping and vice versa for 3g-doping.

We proceed as in Sec. III E to obtain the Jij values

and TC. Postponing a discussion of GdCo5 to the next

section, this analysis for YCo5 reveals two key points.

First, for Ni-doping,J2c−2c,J2c−3g andJ3g−3g only

un-dergo small changes from the pristine case, while the J parameters coupling to Ni are negligible. Therefore the observed reduction inTCwith Ni-doping is essentially a

dilution effect. We recall from Fig. 5 that the interlayer coupling dominates the magnetic properties. Doping on the 2csite therefore has a larger effect onTCsimply due

to the lower multiplicity of this site; taking YCo4Ni as an

example, 2c-doping reduces the cobalt content in a layer by 50% compared to only 33% with 3g-doping. This dif-ference alone can account for a 20 K reduction in TC

moving from 3g to 2c-doping.

The second point applies to the Fe-doped compound YCo4.5Fe0.5. When solving the eigenvalue problem

of equation 9, the eigenvectors give the relative or-dering strengths of the different sublattices. For the cases of 2c and 3g-doping respectively, the normalized (hCo2c, hCo3g, hFe) eigenvectors are (0.49,0.44,0.75) and (0.61,0.55,0.58). That is, for 2c-doping the magnetic or-dering close to TC is dominated by the Fe sublattice,

thanks to a large value ofJFe−Fe (29 mRy). As we

ex-plore in the next section, the presence of Fe at the 2c sites also modifies the exchange field at the RE site.

In Fig. 11 we compare our calculatedTCfor YCo5−xTx

with previously-published experimental data.32,33,35,40 The experiments also find an increase or decrease inTC

for Fe or Ni-doping, respectively. As already noted, the calculatedTC for YCo5 is lower than that measured

ex-perimentally, and the left panel of Fig. 11 also illustrates the scatter in reported experimental values. Therefore in the right panel of Fig. 11 we plot the same data as a difference relative to theTCmeasured for YCo5, and

in-clude our calculated data for 2c or 3g-doping. With the exception of YCo4.5Ni0.5 the experimental data points

fall in between the 2c/3g limiting cases. We tentatively note that the values ofTCof Fe-doped YCo5measured in

pref--1.0 0.0 1.0 700

800 900 1000 1100

Change in electron count w.r.t. YCo_{5}

T (K)C

YCo4Fe YCo4.5Fe0.5 YCo5 YCo4.5Ni0.5YCo4Ni

-1.0 0.0 1.0

-200 -100 0 100 200

Change in electron count w.r.t. YCo_{5}

Δ

T (K)C

YCo4Fe YCo4.5Fe0.5 YCo5 YCo4.5Ni0.5YCo4Ni

FIG. 11. Curie temperatures of doped YCo5, shown on an absolute scale (left panel) or relative to theTCmeasured/calculated

for pristine YCo5 (right panel). The experimentalTCvalues were previously reported in Refs. 40 (diagonal crosses), 33 (filled

squares), 35 (upright crosses) and 32 (asterisks). The right panel additionally shows the calculatedTCvalues for doped YCo5

(cf. Fig. 10) with the dopants at Co2c(circles, dashed lines) or Co3g (empty squares, solid lines) sites.

erential 2csubstitution, which would support the conclu-sion based on ThCo5that 3gsubstitution is preferable.37

However, given the uncertainties in measuring and cal-culatingTCwe acknowledge that such an indirect

assign-ment can only be speculative.

J. Substitutional doping of transition metals IV: Modification of the RE-TM interaction through

doping

Aside from modification of the magnetization andTC,

it is important to establish the effect that substitutional doping has on the RE. For instance, since it is the Sm itself which provides the large anisotropy in SmCo5,7

con-trol of the RE is equivalent to concon-trolling the anisotropy. For the current case, it is important to establish whether the difficulty in synthesizing GdCo4.5Fe0.5has a magnetic

origin. Therefore we use our calculations to investigate the RE-TM interaction in GdCo4.5T0.5for T = Ni, Fe. In

Fig. 12(a) we show the temperature evolution of the Gd magnetization (cf. Fig. 4 for pristine GdCo5) for

preferen-tial 2cor 3g-doping. In Fig. 12(b) we plot the calculated Jij parameters of equation 9 which quantify the RE-TM

interaction.

Focusing on Ni-doping first (left panels of Fig. 12) we find that doping on the 2c site has a negligible effect on the Gd magnetization. Indeed, we find the value of JGd−Ni to be close toJGd−Co2c, despite the weaker mag-netism of Ni. However, doping with Ni on the 3g-site reduces the exchange field at the RE site and causes a faster reduction in the Gd magnetization with temper-ature. Although the value of JGd−Ni calculated for

3g-doping is larger than that calculated for 2c-3g-doping, it is smaller than JGd−Co3g by almost 50%. Given that it is JGd−Co3g which drives the RE ordering (Sec. III D), this reduction has a noticeable effect on the RE magnetiza-tion.

Given that Ni is magnetically weaker than Co, it is not too surprising that we observe a weaker RE-TM in-teraction. Conversely, given that both TC and the zero

temperature magnetization increase with Fe-doping, it is tempting to assume that Fe-doping might strengthen the RE-TM interaction, especially when substituted at 3g sites. However, our calculations (right panel of Fig. 12) do not support this view. Doping at the 3gsite does give a slightly slower decay of the Gd magnetization due to an enhanced value ofJGd−Fe. However, this value is only

6% larger thanJGd−Co3g [filled red bars in Fig. 12(b)], so in GdCo4.5Fe0.5 the effect is minimal.

Surprisingly, our calculations further find that Fe-doping at the 2c-site actually weakens the RE-TM inter-action and causes a faster temperature decay of the Gd magnetization compared to the pristine case [right panel of Fig. 12(a)]. This unexpected result can be traced to a positive value of JGd−Fe, i.e. a ferromagnetic

interac-tion between the RE and the Fe atoms located at the 2c
sites. This finding is robust against the choice of
spheri-cal approximation to the potential (using the muffin-tin
approximation). We note that such a ferromagnetic
in-teraction cannot be accounted for in the standard model
of RE-TM interactions based on the hybridization of
mi-nority TM-3dwith majority RE-5d electrons.6 _{The fact}

that this behavior is only calculated for 2c-doping in-dicates the existence of a secondary effect when the Fe dopants are placed at nearest neighbor positions to the RE. Such competing magnetic interactions will have a detrimental effect on the solubility of Fe. It is interest-ing to note that codopinterest-ing GdCo5 with B stabilizes

com-pounds with higher Fe content, given that B occupies precisely these 2c sites.41

IV. SUMMARY AND CONCLUSIONS

We have studied the RECo5−xTxfamily of compounds

where RE = Y and Gd and T = Ni and Fe. Our purpose was to probe the TM-TM and RE-TM interactions which govern rare-earth/transition-metal permanent magnets, taking advantage of the relatively simple RECo5

0 100 200 300 400 500 600 2.0

4.0 6.0 8.0

T(K)

|M

|(

)

µB

G

d

GdCo4.5Fe0.5

0 100 200 300 400 500 600 2.0

4.0 6.0 8.0

T(K)

|M

|(

)

µB

G

d

GdCo4.5Ni0.5

-10 -5 0 5

J(

m

R

y)

Gd-Co2c Gd-Co3g Gd-Gd Gd-Fe -10

-5 0 5

J(

m

R

y)

Gd-Co2c Gd-Co3g Gd-Gd Gd-Ni

FIG. 12. (a) Absolute magnetization of the Gd sublattice and (b) calculatedJ parameters for Ni or Fe-doped GdCo4.5T0.5.

Doping on the Co2cor Co3g site is denoted in (a) by empty circles and squares, respectively, and by empty and light-filled bars in (b). Dark blue filled circles/bars correspond to pristine GdCo5.

have combined state-of-the-art computational and ex-perimental methods: first-principles calculations based on self-interaction corrected DFT and the disordered lo-cal moment picture to lo-calculate magnetic properties for 0 < T < TC, and single-crystal growth with the optical

floating zone technique to obtain high-quality samples.

Beginning with the pristine YCo5 and GdCo5

com-pounds, we obtained a theoretical interpretation of the experimentally-measured magnetization vs temperature curves. In particular, the calculations explain the oppo-site temperature dependences of the two compounds and the ordering of TC. The increase in GdCo5

magnetiza-tion with temperature was shown to arise from a faster decay of the Gd magnetization compared to Co, while the higherTCof GdCo5 was attributed to both a

modi-fication of the lattice parameters due to the presence of Gd, and also the favorable magnetic coupling between Gd and the Co sublattices. Expanding the potential en-ergy in terms of order parameters showed the dominant magnetic interaction to occur between the planes of the hexagonal CaCu5 structure. Comparison of the

calcu-lated Weiss fields with the exchange field at the RE site
reported from INS measurements76 _{found good }

agree-ment, supporting the application of the DLM picture to this system.

For the doped systems, both experiments and calcula-tions showed an increase or decrease in magnetization with Fe or Ni-substitution, respectively. The calcula-tions found that this change in magnetization did not depend on whether the dopants were placed at the 2c or 3g crystallographic sites. The calculated values of

TC also showed the same increase/decrease for

Fe/Ni-doping, in agreement with previously-published data for

YCo5−xTx.32,33,35,40 However, here a dependence on the

doping site was observed, with larger changes inTC

cal-culated for 2c-doping. For Ni-doping this dependence was explained as a dilution effect, while for Fe-doping the higherTC for the 2c case was found to arise from a

strong Fe-Fe ferromagnetic interaction.

Examining the RE-TM interaction for the doped GdCo5−xTx compounds, substituting Ni at the 3g site

was found to induce a faster reduction in the Gd mag-netization with temperature, as compared to the pristine compound or 2c-doping. However, substituting Fe also showed this faster reduction in magnetization, this time for 2c-doping. The order parameter expansion of the po-tential energy surface traced the origin of this effect to a ferromagnetic coupling between Gd and Fe at the 2c sites.

Aside from these specific findings described above, the current study has laid the necessary groundwork for the further investigation of the full RECo5 family

(e.g. SmCo5), where the RE-CF interactions play a key

role. In particular we have established the viability of the experimental and computational protocols needed to synthesize, characterize and model the RETM5

perma-nent magnets. However, our study has also identified a new avenue of study for GdCo5−xFex regarding the

Gd-Fe(2c) interaction. We have raised the possibility that the experimentally-known41 necessity of codoping GdCo5−xFexwith B is related to the calculated

interac-tions. For Ni-substitution, although in the current study we have focused on low doping concentrations, by extrap-olating the GdCo5 data in Fig 8 to higher Ni-doping we

can expect a switch from TM to Gd-dominated magne-tization at zero temperature, which should yield a com-pensation point. There is also a question of whether the TM-magnetization collapses at a critical concentration of Ni or whether it continuously decreases to zero.54

As a final note, we point out that the current study has focused on magnetization along a single direction and not addressed anisotropic quantities. Aside from the study of pristine YCo5 presented in Ref. 61, there is further work

to be done regarding the doped compounds. More funda-mentally there is the question of the anomalous temper-ature dependence of the magnetocrystalline anisotropy in GdCo5, particularly regarding the role of anisotropic

exchange.21,22,27 Through the combination of our fully-relativistic calculations with high-quality single crystals, we are well-equipped to address such questions in future work.

ACKNOWLEDGMENTS

The present work forms part of the PRETAMAG project, funded by the UK Engineering and Physical Sciences Research Council, Grant no. EP/M028941/1. Work at Daresbury Laboratory was supported by an EP-SRC service level agreement with the Scientific Comput-ing Department of STFC. We acknowledge useful discus-sions with M. Matsumoto, Prof. G. Rowlands, M. Laver, M. Lueders, Z. Szotek and A. Walton. We thank Dr. A. Vasylenko for his assistance in translating Ref. 33, Dr. M. Ciomaga Hatnean for assistance with single crystal growth and D. A. Duncan and O. J. Parish for preparing initial samples of doped RECo5 compounds.

Appendix A: Structural characterization

In Fig. 13 we show the lattice constants a and c of the synthesized (polycrystallline) compounds measured by powder x-ray diffaction at room temperature.

Appendix B: Computational details

Our calculations proceed in two steps. First, a self-consistent, scalar-relativistic calculation is performed on the magnetically-ordered system in order to determine the potentials associated with each atomic species (note that compositionally-disordered systems can be treated at this step with the CPA). Then, these potentials are fed into a non-self-consistent, fully-relativistic CPA calcula-tion to model the magnetically-disordered system whose local moments are orientated according to the probability distribution specified by{λi}.

a (

Å

)

c (

Å

)

4.92 4.94 4.96 4.98

RCo4.5Fe0.5 RCo5 RCo4.5Ni0.5 RCo4Ni

-1.0 0.0 1.0

3.97 3.99 4.01

Change in electron count w.r.t. RCo_{5}

FIG. 13. Lattice parameters (in ˚A) measured by powder x-ray diffraction for the as-cast samples of transition metal-doped YCo5 (green, crosses) and GdCo5 (blue, stars).

For the first step, we use the local-spin-density
approx-imation for the exchange-correlation potential,77
treat-ing the 4f electrons of Gd with the local-self-interaction
correction.68 _{The Kohn-Sham potential is determined}

under a spherical approximation, namely the atomic-sphere approximation (ASA). The ASA atomic-sphere radii at the three distinct crystal sites (RE, TM2c, TM3g) were

(1.84, 1.39, 1.42) ˚A for YTM5and (1.85, 1.39, 1.42) ˚A for

GdTM5. These values were chosen based on the results

of a test calculation performed on YCo5with the

plane-wave projected-augmented plane-wave codeGPAW,78 _{observing}

the radii at which the potentials centered at the three sites showed similar deviations from spherical symmetry subject to the ASA total volume constraint.

We investigated the spherical approximation further by performing calculations under the muffin-tin (MT) ap-proximation for the potential, which prohibits the over-lap of different potential spheres and consequently in-troduces a flat-potential interstitial region. Our calcu-lated critical temperatures based on MT calculations are generally smaller than the ASA ones by ∼100 K, but trends (e.g. the relative critical temperatures of GdCo5

and YCo5, and the effect of doping on different sites)

are preserved. However, the calculated molecular field at the Gd site is smaller in the MT approximation by al-most a factor of 2. Test calculations on the magnetocrys-talline anisotropy also find that the MT approximation fails to predict the experimentally-observed easyc-axis, while the ASA does.48,49,61

spherical harmonics up to a maximum angular momen-tum quanmomen-tum number of l = 3. Although the KKR-CPA is an all-electron method, there is still a partition-ing of electrons into core and valence which determines their treatment within multiple-scattering theory; here the 4p(5p) states were treated as valence for Y (Gd). A 20×20×20 Brillouin zone sampling was used and a fixed electronic temperature of 400 K in calculating the elec-tronic occupations in the self-consistent calculation.

For the second step in our two-step procedure we
solve the fully-relativistic scattering problem80,81 _{using}

the previously-generated “frozen” potentials. Here the k-space integration is performed to high accuracy using an adaptive sampling algorithm.82 The electronic states were populated according to the Fermi-Dirac distribu-tion whose temperature was chosen to match the local moment statistics forT ≥400Kand kept at 300 K other-wise. The integration over angular variables in equation 6 was performed numerically on a 240×40 mesh equally spaced in sinθi and φi, and the necessary energy

inte-grations were performed on a rectangular grid extending
2 Rydbergs into the complex plane, using a logarithmic
spacing with ten points per decade for the legs of the
contour parallel to the imaginary axis. We note that the
calculated electronic density could then be used to
con-struct new potentials in an iterative scheme,83 _{but here}

we keep the potentials frozen in line with the local mo-ment picture.

Since the second part of the calculations is fully-relativistic, the thermally-averaged orbital angular mo-mentumhµorbi0,T can develop a nonzero value. However,

the frozen potentials do not contain any explicit coupling

to orbital angular momentum, e.g. through an
empiri-cal orbital polarization correction (OPC) term.84 _{It has}

been observed that including such a term increases the magnitude of the orbital moments in YCo5 and also of

the anisotropy.48,49,51_{Due to its empirical nature and the}

fact that it is largely untested for magnetically-disordered systems, we choose not to include an OPC term in the current study.

As mentioned in section II D, the Weiss fields appear on both sides of equation 6, since the {λi} values de-termineP0. Following Ref. 61 we obtain the Weiss fields

iteratively. For lower temperatures (λ >_{∼}2) we find an
ap-proach based on fixingT to be efficient, i.e. theλ-values
for the next calculation are obtained from the Weiss fields
of the previous (prev) calculation as

λnext_{i} =βhprev_{i} (B1)

for each sublatticei. For smallerλ-values we find it more efficient to fixλ; i.e. for sublattice i λi is fixed to some

value (2, 1, 0.5, 0.1) and λj updated until a consistent

solution is reached:

λnext_{j} =λi

hprev_{j}

hprev_{i} . (B2)

Finally we note that we have a choice of magnetization
direction through the orientations of{λi}. To make
con-tact with previous work61_{we kept the magnetization }

di-rection fixed along [101] and obtain the hi magnitudes

for the iterative scheme by projecting onto the inputλi direction. We leave the important questions of magne-tocrystalline anisotropy, anisotropic exchange and mag-netization anisotropy21,22,27 for future study.

∗

j.b.staunton@warwick.ac.uk

1 _{K. Strnat, G. Hoffer, J. Olson, W. Ostertag,} _{and J. J.}

Becker, J. Appl. Phys.38, 1001 (1967).

2

J. M. D. Coey, IEEE Trans. Magn.47, 4671 (2011).

3

K. H. J. Buschow, in Handbook of Magnetic Materials, Vol. 10, edited by K. H. J. Buschow (Elsevier B.V., 1997) Chap. 4, p. 463.

4

O. Gutfleisch, M. A. Willard, E. Br¨uck, C. H. Chen, S. G. Sankar, and J. P. Liu, Adv. Mater.23, 821 (2011).

5

M. Richter, J. Phys. D: Appl. Phys.31, 1017 (1998).

6

K. Kumar, J. Appl. Phys.63, R13 (1988).

7 _{A. Ermolenko, IEEE Trans. Magn.}_{12}_{, 992 (1976).}
8

M. D. Kuz’min and A. M. Tishin, inHandbook of Magnetic Materials, Vol. 17, edited by K. H. J. Buschow (Elsevier B.V., 2008) Chap. 3, p. 149.

9 _{A. S. Yermolenko, Fiz. metal. metalloved.}_{50}_{, 741 (1980).}
10

B. L. Gy¨orffy, A. J. Pindor, J. Staunton, G. M. Stocks, and H. Winter, J. Phys. F: Met. Phys.15, 1337 (1985).

11 _{J. J. M. Franse and R. J. Radwa´}_{nski, in}_{Handbook of }
Mag-netic Materials, Vol. 7, edited by K. H. J. Buschow
(Else-vier North-Holland, New York, 1993) Chap. 5, p. 307.

12 _{K. Nassau, L. Cherry, and W. Wallace, J. Phys. Chem.}

Solids16, 131 (1960).

13

E. A. Nesbitt, H. J. Williams, J. H. Wernick, and R. C. Sherwood, J. Appl. Phys.33, 1674 (1962).

14 _{E. Burzo, Phys. Rev. B}_{6}_{, 2882 (1972).}
15

T. Okamoto, H. Fujii, C. Inoue, and E. Tatsumoto, J. Phys. Soc. Japan34, 835 (1973).

16 _{T. Katayama, M. Ohkoshi, Y. Koizumi, T. Shibata, and}

T. Tsushima, Appl. Phys. Lett.28, 635 (1976).

17

M. Uehara, J. Appl. Phys.53, 3730 (1982).

18 _{A. Ermolenko, IEEE Trans. Magn.}_{15}_{, 1765 (1979).}
19

R. Radwa´nski, Physica B+C142, 57 (1986).

20

R. Ballou, J. D´eportes, B. Gorges, R. Lemaire, and J. Ous-set, J. Magn. Magn. Mater.54, 465 (1986).

21

R. Radwa´nski, J. Franse, P. Quang, and F. Kayzel, J. Magn. Magn. Mater.104, 1321 (1992).

22 _{P. Gerard and R. Ballou, J. Magn. Magn. Mater.}_{104}_{, 1463}

(1992).

23

M. D. Kuz’min, Y. Skourski, D. Eckert, M. Richter, K.-H. M¨uller, K. P. Skokov, and I. S. Tereshina, Phys. Rev. B

70, 172412 (2004).

24

W. Frederick and M. Hoch, IEEE Trans. Magn. 10, 733 (1974).

25 _{H. Klein, A. Menth,} _{and R. Perkins, Physica B+C} _{80}_{,}

26

E. Tatsumoto, T. Okamoto, H. Fujii, and C. Inoue, J. Phys. Colloques32, C1 (1971).

27 _{J. M. Alameda, D. Givord, R. Lemaire,} _{and Q. Lu, J.}

Appl. Phys.52, 2079 (1981).

28 _{J. Schweizer and F. Tasset, J. Phys. F: Met. Phys.}_{10}_{, 2799}

(1980).

29

M. Yamaguchi, T. Ohta, and T. Katayama, J. Magn. Magn. Mater.31, 221 (1983).

30 _{J. Miller and A. Austin, J. Crys. Growth}_{18}_{, 7 (1973).}
31

T. Katayama and T. Shibata, J. Crys. Growth 24, 396 (1974).

32 _{K. H. J. Buschow and M. Brouha, J. Appl. Phys.}_{47}_{, 1653}

(1976).

33

A. S. Yermolenko and A. F. Rojda, Fiz. metal. metalloved.

43, 312 (1977).

34

J. Deportes, D. Givord, J. Schweizer, and F. Tasset, IEEE Trans. Magn.12, 1000 (1976).

35 _{Y. Chuang, C. Wu, and Y. Chang, J. Less Common Met.}

84, 201 (1982).

36

V. Crisan, V. Popescu, A. Vernes, D. Andreica, I. Burda, and S. Cristea, J. Alloys Compd.223, 147 (1995).

37 _{J. Laforest and J. Shah, IEEE Trans. Magn.}_{9}_{, 217 (1973).}
38

F. Rothwarf, H. A. Leupold, J. Greedan, W. E. Wallace, and D. K. Das, Int. J. Magnetism4, 267 (1973).

39 _{K. N. R. Taylor and C. A. Poldy, J. Phys. F: Met. Phys.}

5, 1593 (1975).

40

A. Paoluzi, L. Pareti, M. Solzi, and F. Albertini, J. Magn. Magn. Mater.132, 185 (1994).

41

Z. Drzazga, A. Winiarska, and F. Stein, J. Less Common Met.153, L21 (1989).

42 _{J. P. Liu, X. P. Zhong, F. R. de Boer,} _{and K. H. J.}

Buschow, J. Appl. Phys.69, 5536 (1991).

43

J. Franse, N. Thuy, and N. Hong, J. Magn. Magn. Mater.

72, 361 (1988).

44 _{Z. Tie-song, J. Han-min, G. Guang-hua, H. Xiu-feng, and}

C. Hong, Phys. Rev. B43, 8593 (1991).

45

T.-S. Zhao, H.-M. Jin, R. Gr¨ossinger, X.-C. Kou, and H. R. Kirchmayr, J. Appl. Phys.70, 6134 (1991).

46

J. K¨ubler, Theory of Itinerant Electron Magnetism

(Clarendon Press, Oxford, 2000).

47 _{R. Skomski, P. Manchanda, P. Kumar, B. Balamurugan,}

A. Kashyap, and D. J. Sellmyer, IEEE Trans. Magn.49, 3215 (2013).

48 _{L. Nordstrom, M. S. S. Brooks,} _{and B. Johansson, J.}

Phys.: Condens. Matter4, 3261 (1992).

49

G. H. O. Daalderop, P. J. Kelly, and M. F. H. Schuurmans, Phys. Rev. B53, 14415 (1996).

50 _{H. Yamada, K. Terao, F. Ishikawa, M. Yamaguchi, H. }

Mi-tamura, and T. Goto, J. Phys.: Condens. Matter11, 483 (1999).

51 _{L. Steinbeck, M. Richter, and H. Eschrig, Phys. Rev. B}

63, 184431 (2001).

52

K. Uebayashi, K. Terao, and H. Yamada, J. Alloys Compd.

346, 47 (2002).

53

A. Kashyap, R. Skomski, R. F. Sabiryanov, S. S. Jaswal, and D. J. Sellmyer, IEEE Trans. Magn.39, 2908 (2003).

54 _{F. Ishikawa, I. Yamamoto, I. Umehara, M. Yamaguchi,}

M. Bartashevich, H. Mitamura, T. Goto, and H. Yamada, Physica B328, 386 (2003).

55

P. Larson and I. I. Mazin, J. Appl. Phys.93, 6888 (2003).

56 _{P. Larson, I. I. Mazin, and D. A. Papaconstantopoulos,}

Phys. Rev. B69, 134408 (2004).

57

H. Rosner, D. Koudela, U. Schwarz, A. Handstein, M.

Han-fland, I. Opahle, K. Koepernik, M. D. Kuz’min, K.-H. Muller, J. A. Mydosh, and M. Richter, Nature Phys.2, 469 (2006).

58

D. Koudela, U. Schwarz, H. Rosner, U. Burkhardt, A. Handstein, M. Hanfland, M. D. Kuz’min, I. Opahle, K. Koepernik, K.-H. M¨uller, and M. Richter, Phys. Rev. B77, 024411 (2008).

59

D. Benea, O. Isnard, N. Coroian, and V. Pop, J. Magn. Magn. Mater.322, 1052 (2010).

60

X. B. Liu, Z. Altounian, and M. Yue, J. Appl. Phys.107, 09A718 (2010).

61 _{M. Matsumoto, R. Banerjee, and J. B. Staunton, Phys.}

Rev. B90, 054421 (2014).

62

P. Kumar, A. Kashyap, B. Balamurugan, J. E. Shield, D. J. Sellmyer, and R. Skomski, J. Phys.: Condensed Matter

26, 064209 (2014).

63

M. Ochi, R. Arita, M. Matsumoto, H. Kino, and T. Miyake, Phys. Rev. B91, 165137 (2015).

64 _{T. Beuerle, M. Liebs, K. Hummler,} _{and M. F¨}_{ahnle, J.}

Magn. Magn. Mater.132, L1 (1994).

65

J. Liu, F. de Boer, P. de Chˆatel, R. Coehoorn, and K. Buschow, J. Magn. Magn. Mater.132, 159 (1994).

66

B. L. Gy¨orffy and G. M. Stocks, inElectrons in Disordered Metals and at Metallic Surfaces, edited by P. Phariseau and B. Gy¨orffy (Springer US, 1979) Chap. 4, pp. 89–192.

67

H. Ebert, D. K¨odderitzsch, and J. Min´ar, Rep. Prog. Phys.

74, 096501 (2011).

68 _{M. L¨}_{uders, A. Ernst, M. D¨}_{ane, Z. Szotek, A. Svane,}

D. K¨odderitzsch, W. Hergert, B. L. Gy¨orffy, and W. M. Temmerman, Phys. Rev. B71, 205109 (2005).

69 _{J. B. Staunton, L. Szunyogh, A. Buruzs, B. L. Gyorffy,}

S. Ostanin, and L. Udvardi, Phys. Rev. B 74, 144411 (2006).

70

J. B. Staunton, A. Marmodoro, and A. Ernst, J. Phys.: Condens. Matter26, 274210 (2014).

71

S. N. Khan, J. B. Staunton, and G. M. Stocks, Phys. Rev. B93, 054206 (2016).

72 _{K. H. J. Buschow, Rep. Prog. Phys.}_{40}_{, 1179 (1977).}
73

A. Andreev and S. Zadvorkin, Physica B172, 517 (1991).

74

A. V. Andreev, inHandbook of Magnetic Materials, Vol. 8, edited by K. H. J. Buschow (Elsevier North-Holland, New York, 1995) Chap. 2, p. 59.

75

E. Mendive-Tapia and J. B. Staunton, Phys. Rev. Lett.

118, 197202 (2017).

76 _{M. Loewenhaupt, P. Tils, K. Buschow, and R. Eccleston,}

J. Magn. Magn. Mater.138, 52 (1994).

77

S. H. Vosko, L. Wilk, and M. Nusair, Can. J. Phys.58, 1200 (1980).

78

J. Enkovaaraet al., J. Phys.: Condens. Matter22, 253202 (2010).

79 _{M. D¨}_{ane, M. L¨}_{uders, A. Ernst, D. K¨}_{odderitzsch, W. M.}

Temmerman, Z. Szotek, and W. Hergert, J. Phys.: Con-dens. Matter21, 045604 (2009).

80 _{P. Strange, J. Staunton, and B. L. Gyorffy, J. Phys. C:}

Solid State Phys.17, 3355 (1984).

81

P. Strange, H. Ebert, J. B. Staunton, and B. L. Gyorffy, J. Phys.: Condens. Matter1, 2959 (1989).

82 _{E. Bruno and B. Ginatempo, Phys. Rev. B} _{55}_{, 12946}

(1997).

83

A. De´ak, E. Simon, L. Balogh, L. Szunyogh, M. dos San-tos Dias, and J. B. Staunton, Phys. Rev. B 89, 224401 (2014).

84